Chapter 2 A Continuum Damage Model Based on Experiments and Numerical Simulations A Review


 James McGee
 1 years ago
 Views:
Transcription
1 Chapter 2 A Continuum Damage Model Based on Experiments and Numerical Simulations A Review Michael Brünig Abstract The paper summarizes the author s activities in the field of damage mechanics. In this context, a thermodynamically consistent anisotropic continuum damage model is reviewed. The theory is based on consideration of damaged as well as fictitious undamaged configurations. The modular structure of the continuum model is accomplished by kinematic decomposition of strain rates into elastic, plastic and damage parts. A generalized yield condition is used to adequately describe the plastic flow properties of ductile metals and the plastic strain rate tensor is determined by a nonassociated flow rule. Furthermore, a stressstatedependent damage criterion as well as evolution equations of damage strains are proposed. Different branches of the respective criteria are considered corresponding to various damage and failure mechanisms depending on stress state. Since it is not possible to propose and to validate stressstatedependent criteria only based on tests with uniaxially loaded specimens for a wide range of stress states, numerical calculations on the microlevel have been performed to be able to study stressstatedependent mechanisms of microdefects and their effect on macroscopic behavior. In addition, new experiments with twodimensionally loaded specimens have been developed. Corresponding numerical simulations of these experiments show that they cover a wide range of stress triaxialities and Lode parameters in the tension, shear and compression domains. Keywords Ductile damage Stress triaxiality Lode parameter Experiments Numerical simulations M. Brünig (B) Institut Für Mechanik und Statik, Universität der Bundeswehr München, Neubiberg, Germany Springer International Publishing Switzerland 2015 H. Altenbach et al. (eds.), From Creep Damage Mechanics to Homogenization Methods, Advanced Structured Materials 64, DOI / _2 19
2 20 M. Brünig 2.1 Introduction The accurate and realistic modeling of inelastic deformation and failure behavior of engineering materials is essential for the solution of numerous boundaryvalue problems. For example, microscopic defects cause reduction in strength of materials and shorten the life time of engineering structures. Therefore, a main issue in engineering applications is to provide realistic information on the stress distribution within material elements or assessment of safety factors against failure. Continuum damage mechanics analyzes systematically the effect of damage on mechanical properties of materials. Critical values of damage variables can be seen as major parameters at the onset of fracture. An important issue in such phenomenological constitutive approaches is the appropriate choice of the physical nature of mechanical variables characterizing the damage state of materials and their tensorial representation. Therefore, to be able to develop a realistic, accurate and efficient phenomenological model it is important to analyze and to understand the complex stressstatedependent processes of damage and fracture as well as its respective mechanisms acting on different scales. In this context, in the last years various damage models have been published based on experimental observations as well as on multiscale approaches (Brünig 2001, 2003; Gurson 1977; Murakami and Ohno 1981; Lemaitre 1996; Voyiadjis and Kattan 1999). In this context, Brünig et al. (2011b; 2008); Brünig and Gerke (2011) have proposed a generalized and thermodynamically consistent, phenomenological continuum damage model which has been implemented as userdefined material subroutines in commercial finite element programs allowing analyses of static and dynamic problems in differently loaded metal specimens. To be able to detect stress triaxiality dependence of the constitutive equations tension tests with carefully designed specimens have been developed. For example, differently prenotched specimens and corresponding numerical simulations have been used by Bai and Wierzbicki (2008); Bao and Wierzbicki (2004); Becker et al. (1988); Bonora et al. (2005); Brünig et al. (2011b; 2008); Dunand and Mohr (2011); Gao et al. (2010). However, these experiments with unnotched and differently notched flat specimens showed stress triaxialities only in a small region of positive values. Larger triaxialities appear in tension tests with cylindrical (axisymmetric) specimens but they cannot be manufactured when the behavior of thin sheets is investigated. Thus, specimens with new geometries have been designed to be able to analyze stress states with small hydrostatic parts. Tension tests with these specimens have been performed (Bao and Wierzbicki 2004; Gao et al. 2010) leading to shear mechanisms in their centers. Similar specimens have been developed and tested by Brünig et al. (2008); Driemeier et al. (2010). Furthermore, to be able to take into account other regions of stress triaxialities butterfly specimens have been manufactured (Bai and Wierzbicki 2008; Dunand and Mohr 2011; Mohr and Henn 2007) which can be tested in different directions using special experimental equipment. Alternatively, series of new tests with biaxially loaded flat specimens taken from thin sheets have been developed by Brünig et al. (2014a; 2015) leading to
3 2 A Continuum Damage Model Based on Experiments and Numerical Simulations 21 experimental results on inelastic behavior, damage and fracture of ductile metals for a wide range of stress triaxialities not obtained by the experiments discussed above. Further information on damage and failure mechanisms can be obtained by performing numerical simulations on the microlevel (Brocks et al. 1995; Brünig et al. 2011a, 2013, 2014b;Chewetal.2006; Kuna and Sun 1996; Needleman and Kushner 1990; Ohno and Hutchinson 1984; Zhang et al. 2001) considering individual behavior of growth and coalescence of voids and microshearcracks as well as their accumulation to macrocracks. These numerical calculations have been carried out with different loading conditions covering a wide range of macroscopic stress states. The numerical results elucidated which parameters had remarkable effect on macroscopic stressstrain relations and on evolution equations for the damage variables and which ones only had marginal influence. Thus, it was possible to detect different damage mechanisms which have not been exposed by experiments. In the present paper main ideas and fundamental governing equations of the phenomenological continuum damage model proposed by the author are reviewed. Some experimental and numerical results are summarized to demonstrate the efficiency and applicability of the approach. 2.2 Continuum Damage Model Large deformations as well as anisotropic damage and failure of ductile metals are predicted by the continuum model proposed by Brünig (2003) which is based on experimental results and observations as well as on numerical simulations on the microlevel detecting information of microscopic mechanisms due to individual microdefects and their interactions. Similar to the theories presented by Betten (1982); Grabacki (1991); Murakami and Ohno (1981); Voyiadjis and Park (1999) the phenomenological approach is based on the introduction of damaged and corresponding fictitious undamaged configurations and has been implemented into finite element programs. Extended versions of this model (Brünig et al. 2011b, 2008, 2014a, 2015) propose a stressstatedependent damage criterion based on different experiments and data from corresponding numerical simulations. Furthermore, it takes into account numerical results of various analyses using unit cell models (Brünig et al. 2011a, 2013, 2014b). Based on these numerical results covering a wide range of stress states it was possible to propose damage equations as functions of the stress triaxiality and the Lode parameter Kinematics The kinematic approach is based on the introduction of initial, current and elastically unloaded configurations each defined as damaged and fictitious undamaged configurations, respectively (Brünig 2001, 2003). This leads to the multiplicative
4 22 M. Brünig decomposition of the metric transformation tensor Q = R o 1 Q pl R Q el (2.1) where Q describes the total deformation of the material body due to loading, represents the initial damage, Q pl denotes the plastic deformation of the fictitious undamaged body, R characterizes the deformation induced by evolution of damage and Q el represents the elastic deformation of the material body. In addition, the elastic strain tensor A el = 1 2 lnqel (2.2) o R and the damage strain tensor A da = 1 2 ln R (2.3) are introduced. Furthermore, the strain rate tensor Ḣ = 1 2 Q 1 Q (2.4) is defined, which using Eq. (2.1) can be additively decomposed Ḣ = Ḣ el + R 1 H pl R + Q el 1 Ḣ da Q el (2.5) into the elastic the plastic Ḣ el = 1 2 Qel 1 Q el, (2.6) H pl = 1 2 Qel 1 Q pl 1 Q pl Q el, (2.7) and the damage strain rate tensor Ḣ da = 1 R 1 R. (2.8) 2 With the identity (see Brünig (2003) for further details) R Q el = Q el R (2.9) the damage metric transformation tensor with respect to the current loaded configurations, R (see Eq. (2.5)), has been introduced.
5 2 A Continuum Damage Model Based on Experiments and Numerical Simulations Constitutive Equations Dislocations and growth of microdefects are the most common modes of irreversible microstructural deformations at each stage of the loading process. In particular, pure plastic flow is caused by dislocation motion and sliding phenomena along crystallographic planes whereas damagerelated irreversible deformations are due to residual opening of microdefects after unloading. These dissipative processes are distinctly different in their nature as well as in the manner how they affect the compliance of the material and are active on different scales. Consequently, in damagecoupled elasticplastic theories two sets of internal variables corresponding to formation of dislocations (plastic internal variables) as well as to nucleation and growth of microdefects (damage internal variables) are separately used to adequately describe the irreversible constitutive behavior and to compute corresponding strain rate tensors. The effective undamaged configurations are considered to characterize the behavior of the undamaged matrix material. In particular, the elastic behavior of the undamaged matrix material is described by an isotropic hyperelastic law leading to the effective Kirchhoff stress tensor T = 2G A el + (K 23 ) G tra el 1 (2.10) where G and K represent the constant shear and bulk modulus of the undamaged matrix material, respectively, and 1 denotes the second order unit tensor. In addition, onset and continuation of plastic flow of ductile metals is determined a yield criterion. Experiments on the influence of hydrostatic stress on the behavior of metals carried out by Spitzig et al. (1975; 1976) have shown that the flow stress depends approximately linearly on hydrostatic stress. Additional numerical studies performed by Brünig (1999) elucidated that hydrostatic stress terms in the yield condition affect onset of localization and associated deformation modes leading to notable decrease in ductility. Thus, plastic yielding of the matrix material is governed by the DruckerPragertype yield condition f pl ( Ī 1, J 2, c ) = J 2 c ( 1 a ) c Ī1 = 0, (2.11) where Ī 1 = tr T and J 2 = 2 1 dev T dev T denote invariants of the effective stress tensor T, c is the strength coefficient of the matrix material and a represents the hydrostatic stress coefficient. The experiments (Spitzig et al. 1975, 1976) also showed that plastic deformations are nearly isochoric. Thus, the plastic potential function g pl ( T) = J 2 (2.12)
6 24 M. Brünig is assumed to depend only on the second invariant of the effective stress deviator leading to the nonassociated isochoric effective plastic strain rate H pl = λ g pl T = 1 λ 2 dev T = γ N. (2.13) J 2 In Eq. (2.13) λ is a nonnegative scalarvalued factor, N = 1 dev T denotes 2 J 2 the normalized deviatoric stress tensor and γ = N H pl = 1 λ represents the 2 equivalent plastic strain rate measure used in the present continuum model. Furthermore, the damaged configurations are considered to characterize the behavior of anisotropically damaged material samples. In particular, since damage remarkably affects the elastic behavior and leads to material softening, the elastic law of the damaged material sample is expressed in terms of both the elastic and the damage strain tensor, (2.2) and (2.3). The Kirchhoff stress tensor of the ductile damaged metal is given by ( T = 2 G + η 2 tra da) A el + [(K 23 ) G + 2η 1 tra da tra el + η 3 (A da A el)] 1 + η 3 tra el A da + η 4 (A el A da + A da A el) (2.14) where the parameters η 1...η 4 describe the deteriorating effect of damage on the elastic material properties. The parameters η 1 and η 2 are related to the isotropic character of damage whereas η 3 and η 4 correspond to anisotropic evolution of damage. With these additional parameters it is possible to simulate the decreases in Young s modulus, Poisson s ratio, shear and bulk moduli measured in experiments (Brünig 2003). Based on many experiments it is well known that the stress state remarkably affects damage mechanisms occurring in ductile metals which is illustrated in Fig. 2.1 (Brünig et al. 2011a, b). For example, under tension dominated loading conditions (high positive stress triaxialities, η η t ) damage in ductile metals is mainly caused Fig. 2.1 Damage mechanisms depending on stress triaxialities
7 2 A Continuum Damage Model Based on Experiments and Numerical Simulations 25 by nucleation and isotropic growth of voids whereas under shear and compression dominated conditions (negative stress triaxialities, η c η 0) evolution of microshearcracks is the predominant damage mechanism. Between these regions, 0 <η< η t damage is a combination of both basic mechanisms with simultaneous growth of voids and formation of microshearcracks. In addition, no damage occurs in ductile metals for high negative stress triaxialities η<η c. Therefore, to be able to develop a realistic, accurate and efficient phenomenological model it is important to analyze and to understand the complex stressstatedependent processes of damage as well as its respective mechanisms acting on different scales. To model onset and continuation of damage the concept of damage surface is adopted. Following the ideas given in Brünig (2003); Chow and Wang (1987) the damage surface is formulated in stress space at the macroscopic damaged continuum level f da = αi 1 + β J 2 σ = 0 (2.15) with the stress invariants I 1 = trt and J 2 = 2 1 devt devt and the damage threshold σ.ineq.(2.15) the variables α and β represent damage mode parameters depending on the stress intensity (von Mises equivalent stress) σ eq = 3J 2, the stress triaxiality η = σ m σ eq = I 1 3 3J 2 (2.16) with the mean stress σ m = 1/3 I 1 as well as on the Lode parameter ω = 2 T 2 T 1 T 3 T 1 T 3 with T 1 T 2 T 3 (2.17) expressed in terms of the principal stress components T 1, T 2 and T 3. Furthermore, evolution of macroscopic irreversible strains caused by the simultaneous nucleation, growth and coalescence of different microdefects is modeled by a stressstatedependent damage rule. Thus, the damage potential function g da ( T) = g da (I 1, J 2, J 3 ) (2.18) is introduced where T represents the stress tensor formulated in the damaged configuration which is workconjugate to the damage strain rate tensor Ḣ da (see Brünig 2003, for further details) and I 1, J 2 and J 3 are corresponding invariants. This leads to the damage strain rate tensor Ḣ da = μ gda T ( g da = μ I gda J 2 dev T + gda J 3 ) dev S (2.19)
8 26 M. Brünig where μ is a nonnegative scalarvalued factor and dev S = dev T dev T 2 3 J 2 1 (2.20) represents the second order deviatoric stress tensor (Brünig et al. 2013, 2014b). Alternatively, the damage strain rate tensor (2.19) can be written in the form ( Ḣ da = μ ᾱ 1 ) 1 + β N + δ M 3 (2.21) where the normalized deviatoric tensors N = dev T and M = J dev S 2 dev S have been used. In Eq. (2.21) the parameters ᾱ, β and δ are kinematic variables describing the portion of volumetric and isochoric damagebased deformations. The damage rule (2.21) takes into account isotropic and anisotropic parts corresponding to isotropic growth of voids and anisotropic evolution of microshearcracks, respectively. Therefore, both basic damage mechanisms (growth of isotropic voids and evolution of microshearcracks) acting on the microlevel are involved in the damage rule (2.21). 2.3 Uniaxial Tension Tests Uniaxial tension tests with unnotched specimens taken from thin sheets are used to identify basic elasticplastic material parameters appearing in the constitutive equations discussed above. From these experiments equivalent stress equivalent plastic strain curves are easily obtained from loaddisplacement curves as long as the uniaxial stress field remains homogeneous between the clip gauges fixed on the specimens during the tests (Brünig et al. 2011b, 2008). For example, fitting of numerical curves and experimental data for an aluminum alloy leads to Young s modulus E = MPa and Poisson s ratio is taken to be ν = 0.3. In addition, the power law function for the equivalent stress equivalent plastic strain function appearing in the yield criterion (2.11) ( ) H γ n c = c (2.22) nc 0 is used to model the workhardening behavior. Good agreement of experimental data and numerical results is achieved for the initial yield strength c 0 = 175 MPa, the hardening modulus H = 2100 MPa and the hardening exponent n = 0.22 (Brünig et al. 2015). Since uniaxial tension tests with differently prenotched specimens are characterized by different hydrostatic stress states in the small region between the notches (Brünig et al. 2011b, 2008; Driemeier et al. 2010), these experiments can be used to determine the hydrostaticstressdependent parameter a/c appearing in the yield
9 2 A Continuum Damage Model Based on Experiments and Numerical Simulations 27 criterion (2.11). However, in these tests with prenotched specimens stress and strain fields are not homogeneous and only quantities in an average sense can be evaluated from these experiments. Therefore, corresponding finite element simulations of these uniaxial tests have been performed. Comparison of the numerically predicted loaddisplacement curves and the experimental ones leads with an inverse identification procedure to the parameter a/c = MPa 1. Moreover, various parameters corresponding to the damage part of the constitutive model have to be identified. For example, onset of damage is determined by comparison of experimental loaddisplacement curves of the uniaxial tension tests with those predicted by numerical analyses based on the elasticplastic model only (Brünig et al. 2011b, 2015). First deviation of these curves is an indicator of onset of deformationinduced damage. Using this procedure, the damage threshold appearing in the damage condition (2.15) isσ = 300 MPa for the aluminum alloy under investigation. 2.4 Numerical Analyses on the MicroScale Identification of further damage parameters is more complicated because most criteria and evolution equations are motivated by observations on the microlevel. Therefore, stress state dependence of the parameters in the damage condition (2.21) and in the damage rule (2.21) has been studied in detail by Brünig et al. (2013; 2014b) performing numerical simulations with microvoidcontaining representative volume elements under various loading conditions. In particular, the numerical analyses of differently loaded microdefect containing unit cells have been performed using the finite element program ANSYS enhanced by an userdefined material subroutine. One eighth of the symmetric cell model as well as the finite element mesh with Delements of type Solid185 are shown in Fig Various loading conditions with Fig. 2.2 Finite element mesh of one eighth of the unit cell
10 28 M. Brünig principal macroscopic stresses acting on the outer bounds of the representative volume elements are taken into account to be able to cover the wide range of stress triaxiality coefficients (16) η = 1, 2/3, 1/3, 0, 1/3, 2/3, 1, 5/3, 2, 7/3 and 3 as well as of the Lode parameters (2.23) ω = 1, 1/2, 0, 1/2, and 1. In all micromechanical numerical calculations the stress triaxiality coefficient and the Lode parameter are kept constant during the entire loading history of the unit cell to be able to accurately analyze their effect on damage and failure behavior of ductile metals. Based on the numerical results of these unitcell calculations (Brünig et al. 2013) different damage mode parameters have been identified for the aluminum alloy: In particular, the damage mode parameter α (see Eq. (2.15)) is given by { 0 for 1 α(η) = 3 η for η>0 (2.23) whereas β is taken to be the nonnegative function with β(η, ω) = β 0 (η, ω = 0) + β ω (ω) 0, (2.24) β 0 (η) = { 0.45 η for 1 3 η η for η>0 (2.25) and β ω (ω) = ω ω ω. (2.26) This function β(η, ω) is visualized in Fig In addition, based on the results of the unit cell analyses the stressstatedependent parameters ᾱ, β and δ in the damage rule (2.27) have been identified by Brünig et al. (2013). The nonnegative parameter ᾱ 0 characterizing the amount of volumetric damage strain rates caused by isotropic growth of microdefects is given by the relation Fig. 2.3 Damage mode parameter β versus stress triaxiality η and Lode parameter ω
11 2 A Continuum Damage Model Based on Experiments and Numerical Simulations 29 0 for η< η for η 1 ᾱ(η) = η for 1 <η η for 2 <η for η> (2.27) The parameter ᾱ is high for high stress triaxialities, smaller for moderate ones and zero for negative triaxilities. Dependence on the Lode parameter ω has not been revealed by the numerical simulations on the microscale. In addition, the parameter β characterizing the amount of anisotropic isochoric damage strain rates caused by evolution of microshearcracks is given by the relation β(η, ω) = β 0 (η) + f β (η) β ω (ω) (2.28) with η + f β (η) β ω (ω) for η + f β (η) β ω (ω) for 2 β(η, ω) = η for 3 <η η for 2 <η for η> η <η 2 3 (2.29) with and f β (η) = η (2.30) β ω (ω) = 1 ω 2. (2.31) The parameter δ also corresponding to the anisotropic damage strain rates caused by the formation of microshearcracks is given by the relation with δ(η, ω) = f δ (η) δ ω (ω) (2.32) { ( η)(1 ω δ(η, ω) = 2 ) for 0 for η> η 2 3 (2.33) It is worthy to note that this parameter δ only exists for small stress triaxialities and mainly depends on the Lode parameter ω. Although its magnitude is small in comparison to the parameters ᾱ and β its effect on the evolution of macroscopic damage strain rates Ḣ da is not marginal (Brünig et al. 2013).
12 30 M. Brünig 2.5 Experiments and Numerical Simulations with Biaxially Loaded Specimens The damage related functions discussed above are only based on numerical calculations on the microlevel and their validation has to be realized by experiments also covering a wide range of stress states. This is not possible by the uniaxial tests mentioned above and, therefore, new experiments with biaxially loaded specimens have been developed by Brünig et al. (2014a; 2015). The experiments are performed using the biaxial test machine (Type LFMBIAX 20 kn from Walter Bai, Switzerland) shown in Fig It is composed of four electromechanically, individually driven cylinders with load maxima and minima of ±20 kn (tension and compression loading is possible). The specimens are fixed in the four heads of the cylinders where clamped or hinged boundary conditions are possible. The geometry of the flat specimens and the loading conditions are shown in Fig The load F 1 will lead to shear mechanisms in the center of the specimen whereas simultaneous loading with F 2 leads to superimposed tension or compression modes leading to sheartension or shearcompression deformation and failure modes. Therefore, these tests cover the full range of stress states corresponding to the damage and failure mechanisms discussed above with focus on high positive as well as low positive, nearly zero and negative stress triaxialities. Figure 2.6 clearly shows that different load ratios F 1 : F 2 have remarkable influence on the damage and final fracture modes. For example, for the tension test without Fig. 2.4 Biaxial test machine
13 2 A Continuum Damage Model Based on Experiments and Numerical Simulations 31 Fig. 2.5 Specimen and loading conditions shear loading, F 1 : F 2 = 0 : 1, a nearly vertical fracture line is obtained. Under this loading condition, damage is mainly caused by growth and coalescence of voids with small influence of microshearcracks leading to the macroscopic tensile fracture mode with small cupcone fracture effect (Fig. 2.6a). On the other hand, for pure shear loading, F 1 : F 2 = 1 : 0, shear fracture is observed where the fracture line has an angle of about 25 with respect to the vertical line. Under this loading condition, damage is mainly caused by formation of microshearcracks leading to the macroshearcrack shown in Fig. 2.6b. For sheartension loading, F 1 : F 2 = 1 : 0.5, sheartension fracture is obtained and the fracture line has an angle of only about 10 with respect to the vertical line. Under this loading condition, damage is caused by the simultaneous growth of voids and formation of microshearcracks leading to the macroscopic fracture mode shown in Fig. 2.6c which is between tensile fracture (Fig. 2.6a) and shear fracture (Fig. 2.6b). However, for shearcompression loading, F 1 : F 2 = 1 : 0.5, again shear fracture is observed and the fracture line again has an angle of about 25 with respect to the vertical line. Under this loading condition damage seems to be caused only by formation of microshearcracks leading to the macroshearcrack shown in Fig. 2.6d. It is worthy to note that the damage and failure mechanisms for F 1 : F 2 = 1 : 0 (Fig. 2.6b) and F 1 : F 2 = 1 : 0.5(Fig. 2.6d) seem to be very similar and damage modes characteristic for shear loading will not be remarkably affected by superimposed small compression loads. Furthermore, corresponding numerical simulations have been performed to be able to get detailed information on amounts and distributions of different stress and strain measures as well as further parameters of interest especially in critical regions (Brünig et al. 2015). For example, numerically predicted distributions of the stress triaxiality η at the onset of damage are shown in Fig. 2.7 for different load ratios. In particular, for uniaxial tension loading F 1 : F 2 = 0 : 1 remarkable high stress triaxialities up to η = 0.84 are numerically predicted in the center of the specimen. These high values are caused by the notches in horizontal and thickness direction
14 32 M. Brünig Fig. 2.6 Fracture modes of differently loaded specimens: a F 1 : F 2 = 0 : 1, b F 1 : F 2 = 1 : 0, c F 1 : F 2 = 1 : 0.5, d F 1 : F 2 = 1 : 0.5 Fig. 2.7 Distribution of the stress triaxiality η for different load ratios leading to high hydrostatic stress during elongation of the specimen. This will lead to damage and failure mainly due to growth of voids. In addition, when the specimen is only loaded by F 1 : F 2 = 1 : 0 (shear loading condition) the stress triaxiality η is numerically predicted to be nearly zero in the whole vertical section shown in Fig. 2.7.
15 2 A Continuum Damage Model Based on Experiments and Numerical Simulations 33 Thus, damage will start in the specimen s center and will be caused by formation and growth of microshearcracks. Furthermore, combined loading in vertical and horizontal direction, F 1 and F 2, will lead to combination of these basic damage modes. For example, for the load ratio F 1 : F 2 = 1 : 1 the stress triaxiality is again nearly constant in the vertical section with η = 0.25, and very similar distribution is numerically predicted for F 1 : F 2 = 1 : 0.5 with η = On the other hand, the load ratio F 1 : F 2 = 1 : 0.5 represents combined shearcompression loading with the stress triaxiality η = 0.14 which is nearly constant in the vertical section shown in Fig For this negative stress triaxiality η damage and failure will be caused by formation and growth of microshearcracks only. These numerical results nicely correspond to the fracture modes discussed above and shown in Fig The stress triaxialities η covered by experiments with different flat specimens manufactured from thin sheets are shown in Fig In particular, for unnotched dogboneshape specimens (green) nearly homogeneous stress states occur in the small part during uniaxial tension tests with stress triaxiality η = 1/3. Higher stress triaxialities can be obtained in uniaxial tension tests when notches with different radii are added in the middle part of the specimens (red). Decrease in notch radius will lead to an increase in stress triaxiality in the specimen s center up to η = 1/ 3. In addition, shear specimens (blue) elongated in uniaxial tension test will lead to stress triaxialities of about η = 0.1 when notches in thickness direction are added in the central part (Brünig et al. 2011b, 2008; Driemeier et al. 2010) whereas without additional notch they will also lead to onset of damage at nearly η = 1/3. However, with these flat specimens taken from thin sheets elongated in uniaxial tension tests only the stress triaxialities shown in Fig. 2.8 (green, red and blue points) can be taken into account whereas no information is obtained for high positive (η >1/ 3), low positive (between 0.1 < η < 1/3) or negative stress triaxialities (η < 0). However, further experiments with new specimens (grey) tested under biaxial loading conditions will lead to stress triaxialities in the requested regimes. The grey points shown in Fig. 2.8 correspond to the loading conditions discussed above but variation Fig. 2.8 Stress triaxialities covered by different specimens
16 34 M. Brünig of the load ratios F 1 : F 2 may lead to stress triaxialities marked by the grey zone shown in Fig Therefore, biaxial tests with 2D specimens discussed above cover a wide range of stress triaxialities and Lode parameters. 2.6 Conclusions The author s activities in the field of damage mechanics have been summarized. The continuum model taking into account stressstatedependent damage criteria and damage evolution laws has been reviewed. Elasticplastic material parameters as well as onset of damage have been identified by uniaxial tension tests with smooth and prenotched flat specimens and corresponding numerical simulations. Further damage parameters depending on stress triaxiality and Lode parameter have been determined using numerical results from unitcell calculations on the microlevel. Since the proposed functions are only based on numerical analyses validation of the stressstatedependent model was required. In this context, a series of experiments with biaxially loaded specimens has been presented. Different load ratios led to sheartension and shearcompression mechanisms with different fracture modes. Corresponding finite element simulations of the experiments revealed a wide range of stress states covered by the tests depending on biaxial loading conditions. They could be used to validate the proposed stressstatedependent functions of the continuum model. References Bai Y, Wierzbicki T (2008) A new model of metal plasticity and fracture with pressure and Lode dependence. Int J Plast 24: Bao Y, Wierzbicki T (2004) On the fracture locus in the equivalent strain and stress triaxiality space. Int J Mech Sci 46:81 98 Becker R, Needleman A, Richmond O, Tvergaard V (1988) Void growth and failure in notched bars. J Mech Phys Solids 36: Betten J (1982) Netstress analysis in creep mechanics. IngenieurArchiv 52: Bonora N, Gentile D, Pirondi A, Newaz G (2005) Ductile damage evolution under triaxial state of stress: theory and experiments. Int J Plast 21: Brocks W, Sun DZ, Hönig A (1995) Verification of the transferability of micromechanical parameters by cell model calculations with viscoplastic material. Int J Plast 11: Brünig M (1999) Numerical simulation of the large elasticplastic deformation behavior of hydrostatic stresssensitive solids. Int J Plast 15: Brünig M (2001) A framework for large strain elasticplastic damage mechanics based on metric transformations. Int J Eng Sci 39: Brünig M (2003) An anisotropic ductile damage model based on irreversible thermodynamics. Int J Plast 19: Brünig M, Gerke S (2011) Simulation of damage evolution in ductile metals undergoing dynamic loading conditions. Int J Plast 27:
17 2 A Continuum Damage Model Based on Experiments and Numerical Simulations 35 Brünig M, Chyra O, Albrecht D, Driemeier L, Alves M (2008) A ductile damage criterion at various stress triaxialities. Int J Plast 24: Brünig M, Albrecht D, Gerke S (2011a) Modeling of ductile damage and fracture behavior based on different micromechanisms. Int J Damage Mech 20: Brünig M, Albrecht D, Gerke S (2011b) Numerical analyses of stresstriaxialitydependent inelastic deformation behavior of aluminum alloys. Int J Damage Mech 20: Brünig M, Gerke S, Hagenbrock V (2013) Micromechanical studies on the effect of the stress triaxiality and the Lode parameter on ductile damage. Int J Plast 50:49 65 Brünig M, Gerke S, Brenner D (2014a) New 2Dexperiments and numerical simulations on stressstatedependence of ductile damage and failure. Procedia Mater Sci 3: Brünig M, Gerke S, Hagenbrock V (2014b) Stressstatedependence of damage strain rate tensors caused by growth and coalescence of microdefects. Int J Plast 63:49 63 Brünig M, Gerke S, Brenner D (2015) Experiments and numerical simulations on stressstatedependence of ductile damage criteria. In: Altenbach H, Brünig M (eds) Inelastic behavior of materials and structures under monotonic and cyclic loading. Advanced Structured Materials Springer, Heidelberg, pp Chew H, Guo T, Cheng L (2006) Effects of pressuresensitivity and plastic dilatancy on void growth and interaction. Int J Solids Struct 43: Chow C, Wang J (1987) An anisotropic theory of continuum damage mechanics for ductile fracture. Eng Fracture Mech 27: Driemeier L, Brünig M, Micheli G, Alves M (2010) Experiments on stresstriaxiality dependence of mterial behavior of aluminum alloys. Mech Mater 42: Dunand M, Mohr D (2011) On the predictive capabilities of the shear modified Gurson and the modified MohrCoulomb fracture models over a wide range of stress triaxialities and Lode angles. J Mech Phys Solids 59: Gao X, Zhang G, Roe C (2010) A study on the effect of the stress state on ductile fracture. Int J Damage Mech 19:75 94 Grabacki J (1991) On some desciption of damage processes. Eur J Mech A/Solids 10: Gurson AL (1977) Continuum theory of ductile rupture by void nucleation and growth: part I yield criteria and flow rules for porous ductile media. J Eng Mater Technol 99:2 15 Kuna M, Sun D (1996) Threedimensional cell model analyses of void growth in ductile materials. Int J Fracture 81: Lemaitre J (1996) A course damage mechanics. Springer, Heidelberg Mohr D, Henn S (2007) Calibration of stresstriaxiality dependent crack formation criteria: a new hybrid experimentalnumerical method. Exp Mech 47: Murakami S, Ohno N (1981) A continuum theory of creep and creep damage. In: Ponter ARS, Hayhorst DR (eds) Creep in structures. Springer, Berlin, pp Needleman A, Kushner A (1990) An analysis of void distribution effects on plastic flow in porous solids. Eur J Mech A/Solids 9: Ohno N, Hutchinson J (1984) Plastic flow localization due to nonuniform void distribution. J Mech Phys Solids 32:63 85 Spitzig WA, Sober RJ, Richmond O (1975) Pressure dependence of yielding and associated volume expansion in tempered martensite. Acta Metallurgica 23: Spitzig WA, Sober RJ, Richmond O (1976) The effect of hydrostatic pressure on the deformation behaviour of maraging and HY80 steels and its implications for plasticity theory. Met Trans 7A: Voyiadjis G, Kattan P (1999) Advances in damage mechanics: metals and metal matrix composites. Elsevier, Amsterdam Voyiadjis G, Park T (1999) The kinematics of damage for finitestrain elastoplastic solids. Int J Eng Sci 37: Zhang K, Bai J, Francois D (2001) Numerical analysis of the influence of the Lode parameter on void growth. Int J Solids Struct 38:
18
Multiscale modeling of failure in ABS materials
Institute of Mechanics Multiscale modeling of failure in ABS materials Martin Helbig, Thomas Seelig 15. International Conference on Deformation, Yield and Fracture of Polymers Kerkrade, April 2012 Institute
More informationANSYS Mechanical Basic Structural Nonlinearities
Lecture 4 Rate Independent Plasticity ANSYS Mechanical Basic Structural Nonlinearities 1 Chapter Overview The following will be covered in this Chapter: A. Background Elasticity/Plasticity B. Yield Criteria
More informationA variational void coalescence model for ductile metals
DOI 1.17/s466116399 ORIGINAL PAPER A variational void coalescence model for ductile metals Amir Siddiq Roman Arciniega Tamer El Sayed Received: 21 February 211 / Accepted: 22 July 211 SpringerVerlag
More informationConstitutive models: Incremental (Hypoelastic) Stress Strain relations. and
Constitutive models: Incremental (Hypoelastic) Stress Strain relations Example 5: an incremental relation based on hyperelasticity strain energy density function and 14.11.2007 1 Constitutive models:
More informationRecent Developments in Damage and Failure Modeling with LSDYNA
Recent evelopments in amage and Failure Modeling with LSYNA r. André Haufe ynamore GmbH Frieder Neukamm, r. Markus Feucht aimler AG Paul ubois Consultant r. Thomas Borvall ERAB 1 Technological challenges
More informationEffective elastic moduli of two dimensional solids with distributed cohesive microcracks
European Journal of Mechanics A/Solids 23 (2004) 925 933 Effective elastic moduli of two dimensional solids with distributed cohesive microcracks Shaofan Li a,, Gang Wang a, Elise Morgan b a Department
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationReference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity",
Reference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity", Oxford University Press, Oxford. J. Lubliner, "Plasticity
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationConstitutive and Damage Accumulation Modeling
Workshop on Modeling and Data needs for LeadFree Solders Sponsored by NEMI, NIST, NSF, and TMS February 15, 001 New Orleans, LA Constitutive and Damage Accumulation Modeling Leon M. Keer Northwestern
More informationConstitutive models: Incremental plasticity Drücker s postulate
Constitutive models: Incremental plasticity Drücker s postulate if consistency condition associated plastic law, associated plasticity  plastic flow law associated with the limit (loading) surface Prager
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationBulk Metal Forming II
Bulk Metal Forming II Simulation Techniques in Manufacturing Technology Lecture 2 Laboratory for Machine Tools and Production Engineering Chair of Manufacturing Technology Prof. Dr.Ing. Dr.Ing. E.h.
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationNUMERICAL SIMULATIONS OF CORNERS IN RC FRAMES USING STRUTANDTIE METHOD AND CDP MODEL
Numerical simulations of corners in RC frames using StrutandTie Method and CDP model XIII International Conference on Computational Plasticity. Fundamentals and Applications COMPLAS XIII E. Oñate, D.R.J.
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More informationSSNV221 Hydrostatic test with a behavior DRUCK_PRAGER linear and parabolic
Titre : SSNV221  Essai hydrostatique avec un comportement[...] Date : 08/08/2011 Page : 1/10 SSNV221 Hydrostatic test with a behavior DRUCK_PRAGER linear and parabolic Summary: The case test proposes
More informationAnisotropic damage evolution in shock waveloaded viscoplastic plates
Arch. Mech., 6, 4, pp. 285 3, Warszawa 28 SIXTY YEARS OF THE ARCHIVES OF MECHANICS Anisotropic damage evolution in shock waveloaded viscoplastic plates M. STOFFEL Institut für Allgemeine Mechanik, RWTH
More informationOn fracture locus in the equivalent strain and stress triaxiality space
International Journal of Mechanical Sciences 46 (2004) 81 98 On fracture locus in the equivalent strain and stress triaxiality space Yingbin Bao, Tomasz Wierzbicki Impact and Crashworthiness Laboratory,
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationLecture #10: Anisotropic plasticity Crashworthiness Basics of shell elements
Lecture #10: 1510735: Dynamic behavior of materials and structures Anisotropic plasticity Crashworthiness Basics of shell elements by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering,
More informationCDPM2: A damageplasticity approach to modelling the failure of concrete
CDPM2: A damageplasticity approach to modelling the failure of concrete Peter Grassl 1, Dimitrios Xenos 1, Ulrika Nyström 2, Rasmus Rempling 2, Kent Gylltoft 2 arxiv:1307.6998v1 [condmat.mtrlsci] 26
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationMODELING OF ELASTOPLASTIC MATERIALS IN FINITE ELEMENT METHOD
MODELING OF ELASTOPLASTIC MATERIALS IN FINITE ELEMENT METHOD Andrzej Skrzat, Rzeszow University of Technology, Powst. Warszawy 8, Rzeszow, Poland Abstract: Userdefined material models which can be used
More informationModification of the Gurson Model for shear failure
European Journal of Mechanics A/Solids 27 (2008) 1 17 Modification of the Gurson Model for shear failure K. Nahshon, J.W. Hutchinson School of Engineering and Applied Sciences, Harvard University, Cambridge,
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationA simple elastoplastic model for soils and soft rocks
A simple elastoplastic model for soils and soft rocks A SIMPLE ELASTOPLASTIC MODEL FOR SOILS AND SOFT ROCKS by Roberto Nova Milan University of Technology 1. MODEL HISTORY The model is the result of the
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationIMECE CRACK TUNNELING: EFFECT OF STRESS CONSTRAINT
Proceedings of IMECE04 2004 ASME International Mechanical Engineering Congress November 1320, 2004, Anaheim, California USA IMECE200460700 CRACK TUNNELING: EFFECT OF STRESS CONSTRAINT Jianzheng Zuo Department
More informationThe Frictional Regime
The Frictional Regime Processes in Structural Geology & Tectonics Ben van der Pluijm WW Norton+Authors, unless noted otherwise 1/25/2016 10:08 AM We Discuss The Frictional Regime Processes of Brittle Deformation
More informationLinear and Nonlinear Analysis of High Dynamic Impact Events with Creo Simulate and Abaqus/Explicit
Linear and Nonlinear Analysis of High Dynamic Impact Events with Creo Simulate and Abaqus/Explicit SAXSIM 2015, TU Chemnitz Dr.Ing. Roland Jakel At a glance: Altran, a global leader 20+ Countries 23,000+
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationBone Tissue Mechanics
Bone Tissue Mechanics João Folgado Paulo R. Fernandes Instituto Superior Técnico, 2016 PART 1 and 2 Introduction The objective of this course is to study basic concepts on hard tissue mechanics. Hard tissue
More informationCohesive band model: a triaxialitydependent cohesive model for damage to crack transition in a nonlocal implicit discontinuous Galerkin framework
University of Liège Aerospace & Mechanical Engineering Cohesive band model: a triaxialitydependent cohesive model for damage to crack transition in a nonlocal implicit discontinuous Galerkin framework
More informationBrittle Deformation. Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm
Lecture 6 Brittle Deformation Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm WW Norton, unless noted otherwise Brittle deformation EarthStructure (2 nd
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationINVERSE METHOD FOR FLOW STRESS PARAMETERS IDENTIFICATION OF TUBE BULGE HYDROFORMING CONSIDERING ANISOTROPY
7 th EUROMECH Solid Mechanics Conference J. Ambrósio et.al. (eds.) Lisbon, Portugal, September 711, 2009 INVERSE METHOD FOR FLOW STRESS PARAMETERS IDENTIFICATION OF TUBE BULGE HYDROFORMING CONSIDERING
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationWellbore stability analysis in porous carbonate rocks using cap models
Wellbore stability analysis in porous carbonate rocks using cap models L. C. Coelho 1, A. C. Soares 2, N. F. F. Ebecken 1, J. L. D. Alves 1 & L. Landau 1 1 COPPE/Federal University of Rio de Janeiro, Brazil
More informationUnified Constitutive Model for Engineering Pavement Materials and Computer Applications. University of Illinois 12 February 2009
Unified Constitutive Model for Engineering Pavement Materials and Computer Applications Chandrakant S. Desai Kent Distinguished i Lecture University of Illinois 12 February 2009 Participation in Pavements.
More informationThe Influence of Strain Amplitude, Temperature and Frequency on Complex Shear Moduli of Polymer Materials under Kinematic Harmonic Loading
Mechanics and Mechanical Engineering Vol. 21, No. 1 (2017) 157 170 c Lodz University of Technology The Influence of Strain Amplitude, Temperature and Frequency on Complex Shear Moduli of Polymer Materials
More informationConcept Question Comment on the general features of the stressstrain response under this loading condition for both types of materials
Module 5 Material failure Learning Objectives review the basic characteristics of the uniaxial stressstrain curves of ductile and brittle materials understand the need to develop failure criteria for
More informationComputers and Geotechnics
Computers and Geotechnics 39 (212) 16 Contents lists available at SciVerse ScienceDirect Computers and Geotechnics journal homepage: www.elsevier.com/locate/compgeo Numerical analysis of the failure process
More informationModelling Progressive Failure with MPM
Modelling Progressive Failure with MPM A. Yerro, E. Alonso & N. Pinyol Department of Geotechnical Engineering and Geosciences, UPC, Barcelona, Spain ABSTRACT: In this work, the progressive failure phenomenon
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationCrack Tip Plastic Zone under Mode I Loading and the Nonsingular T zz stress
Crack Tip Plastic Zone under Mode Loading and the Nonsingular T stress Yu.G. Matvienko Mechanical Engineering Research nstitute of the Russian Academy of Sciences Email: ygmatvienko@gmail.com Abstract:
More informationLowCycle Fatigue Crack Growth in Ti6242 at Elevated Temperature Rebecka Brommesson 1,a, Magnus Hörnqvist,2,b, and Magnus Ekh 3,c
LowCycle Fatigue Crack Growth in Ti6242 at Elevated Temperature Rebecka Brommesson 1,a, Magnus Hörnqvist,2,b, and Magnus Ekh 3,c 1,3 Department of Applied Mechanics, Chalmers University of Technology,
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationStrength of Adhesive Joints: A Parametric Study
Project PAJex1  Report 3 Strength of Adhesive Joints: A Parametric Study W R Broughton, L E Crocker and J M Urquhart July 2001 NPL Materials Centre National Physical Laboratory NPL Report MATC(A)27 July
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More informationSimulation of Thermomechanical Couplings of Viscoelastic Materials
Simulation of Thermomechanical Couplings of Viscoelastic Materials Frank Neff 1, Thomas Miquel 2, Michael Johlitz 1, Alexander Lion 1 1 Institute of Mechanics Faculty for Aerospace Engineering Universität
More informationNonlinear Analysis of Reinforced Concrete Shells Subjected to Impact Loads
Transactions of the 7 th International Conference on Structural Mechanics in Reactor Technology (SMiRT 7) Prague, Czech Republic, August 7, 00 Paper # J0 Nonlinear Analysis of Reinforced Concrete Shells
More informationEvaluation of Material Models to Predict Material Failure in LSDYNA
Department of Construction Sciences Solid Mechanics ISRN LUTFD2/TFHF16/5209SE(155) Evaluation of Material Models to Predict Material Failure in LSDYNA Master s Dissertation by Hjalmar Sandberg Oscar
More informationThe design of a formula student front impact attenuator
The design of a formula student front impact attenuator J.M.J. Schormans MT 10.06 Supervisors: dr. ir. Varvara Kouznetsova Eindhoven University of Technology Department of Mechanical Engineering Computational
More informationDamage MechanicsBased Models for HighCycle Fatigue Life Prediction of Metals
Damage MechanicsBased Models for HighCycle Fatigue Life Prediction of Metals H.A.F. Argente dos Santos (Postdoc Fellow) Dipartimento di Meccanica Strutturale Università degli Studi di Pavia Pavia, December
More informationDevelopment, implementation and Validation of 3D Failure Model for Aluminium 2024 for High Speed Impact Applications
Development, implementation and Validation of D Failure Model for Aluminium 2024 for High Speed Impact Applications Paul Du Bois, Murat Buyuk, Jeanne He, Steve Kan NCACGWU th International LSDYNA Users
More informationAnisotropy and Failure Modeling for Nonlinear Strain. Paths and Its Application to Rigid Packaging. Robert Earl Dick (B.S.C.E, M.S.C.
Anisotropy and Failure Modeling for Nonlinear Strain Paths and Its Application to Rigid Packaging by Robert Earl Dick (B.S.C.E, M.S.C.E) Advisor: Jeong Whan Yoon Submitted in fulfillment of the requirements
More informationContinuum mechanics V. Constitutive equations. 1. Constitutive equation: definition and basic axioms
Continuum mechanics office Math 0.107 ales.janka@unifr.ch http://perso.unifr.ch/ales.janka/mechanics Mars 16, 2011, Université de Fribourg 1. Constitutive equation: definition and basic axioms Constitutive
More informationTheory of Plasticity. Lecture Notes
Theory of Plasticity Lecture Notes Spring 2012 Contents I Theory of Plasticity 1 1 Mechanical Theory of Plasticity 2 1.1 Field Equations for A Mechanical Theory.................... 2 1.1.1 Straindisplacement
More informationIdentification of the plastic zone using digital image correlation
M. Rossi et alii, Frattura ed Integrità Strutturale, 3 (4) 55557; DOI:.3/IGFESIS.3.66 Focussed on: Fracture and Structural Integrity related Issues Identification of the plastic zone using digital image
More informationDynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models
Dynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models I. Rhee, K.J. Willam, B.P. Shing, University of Colorado at Boulder ABSTRACT: This paper examines the global
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationDAMAGE MODEL FOR CONCRETE INCLUDING RESIDUAL HYSTERETIC LOOPS: APPLICATION TO SEISMIC AND DYNAMIC LOADING
Fracture Mechanics of Concrete Structures Proceedings FRAMCOS3 AEDIFICA TIO Publishers, D79104 Frei burg, Germany DAMAGE MODEL FOR CONCRETE INCLUDING RESIDUAL HYSTERETIC LOOPS: APPLICATION TO SEISMIC
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationStrainBased Design Model for FRPConfined Concrete Columns
SP230 57 StrainBased Design Model for FRPConfined Concrete Columns by N. Saenz and C.P. Pantelides Synopsis: A constitutive strainbased confinement model is developed herein for circular concrete columns
More informationModelling the excavation damaged zone in CallovoOxfordian claystone with strain localisation
Modelling the excavation damaged zone in CallovoOxfordian claystone with strain localisation B. Pardoen  F. Collin  S. Levasseur  R. Charlier Université de Liège ArGEnCo ALERT Workshop 2012 Aussois,
More informationPREDICTION OF FATIGUE LIFE OF COLD FORGING TOOLS BY FE SIMULATION AND COMPARISON OF APPLICABILITY OF DIFFERENT DAMAGE MODELS
PREDICTION OF FATIGUE LIFE OF COLD FORGING TOOLS BY FE SIMULATION AND COMPARISON OF APPLICABILITY OF DIFFERENT DAMAGE MODELS M. Meidert and C. Walter Thyssen/Krupp Presta AG Liechtenstein FL9492 Eschen
More informationICES REPORT June The Institute for Computational Engineering and Sciences The University of Texas at Austin Austin, Texas 78712
ICES REPORT 1615 June 2016 A phasefield formulation for fracture in ductile materials: Finite deformation balance law derivation, plastic degradation, and stress triaxiality effects by Michael J. Borden,
More informationEffects of geometry and properties of fibre and matrix on overall. composite parameters
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR Under Creative Commons License 3.0 editorial@ijaser.com Research article
More informationStress Integration for the DruckerPrager Material Model Without Hardening Using the Incremental Plasticity Theory
Journal of the Serbian Society for Computational Mechanics / Vol. / No., 008 / pp. 8089 UDC: 59.74:004.0 Stress Integration for the Druckerrager Material Model Without Hardening Using the Incremental
More informationScienceDirect. Bauschinger effect during unloading of coldrolled copper alloy sheet and its influence on springback deformation after Ubending
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 81 (2014 ) 969 974 11th International Conference on Technology of Plasticity, ICTP 2014, 1924 October 2014, Nagoya Congress
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationElastic Stress Ratchetting and Corotational Stress Rates
TECHNISCHE MECHANIK, Band 23, Heft 24, (23), 92 12 Manuskripteingang: 28. April 23 Elastic Stress Ratchetting and Corotational Stress Rates A. Meyers, H. Xiao and O. Bruhns In memory of Jürgen Olschewski
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More informationsottotitolo Department of Civil and Environmental Engineering
A thirtyyear Titolo survey presentazione of Microplane Models sottotitolo Milano, Dr. Giovanni XX mese Di Luzio 20XX Department of Civil and Environmental Engineering Origin of microplane models Slip
More informationDelamination in the scoring and folding of paperboard
PEERREVIEWED CONVERTING Delamination in the scoring and folding of paperboard DOEUNG D. CHOI, SERGIY A. LAVRYKOV, and BANDARU V. RAMARAO ABSTRACT: Delamination between layers occurs during the creasing
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationSTRESS DROP AS A RESULT OF SPLITTING, BRITTLE AND TRANSITIONAL FAULTING OF ROCK SAMPLES IN UNIAXIAL AND TRIAXIAL COMPRESSION TESTS
Studia Geotechnica et Mechanica, Vol. 37, No. 1, 2015 DOI: 10.1515/sgem20150003 STRESS DROP AS A RESULT OF SPLITTING, BRITTLE AND TRANSITIONAL FAULTING OF ROCK SAMPLES IN UNIAXIAL AND TRIAXIAL COMPRESSION
More informationDynamic behavior of concrete at high strain rates and pressures: II. numerical simulation
International Journal of Impact Engineering 25 (2001) 887 910 Dynamic behavior of concrete at high strain rates and pressures: II. numerical simulation S.W. Park 1, Q. Xia, M. Zhou* The George W. Woodruff
More informationFE FORMULATIONS FOR PLASTICITY
G These slides are designed based on the book: Finite Elements in Plasticity Theory and Practice, D.R.J. Owen and E. Hinton, 1970, Pineridge Press Ltd., Swansea, UK. 1 Course Content: A INTRODUCTION AND
More informationApplication of Three Dimensional Failure Criteria on HighPorosity Chalk
, 56 May 00, Trondheim, Norway Nordic Energy Research Programme Norwegian U. of Science and Technology Application of Three Dimensional Failure Criteria on HighPorosity Chalk Roar Egil Flatebø and Rasmus
More information*MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials
14 th International LSDYNA Users Conference Session: Constitutive Modeling *MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials Jesper Karlsson 1, Mikael Schill 1, Johan Tryding
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More informationPREPARATION OF HEXCALIBER TESTS AND PRELIMINARY THERMOMECHANICAL ANALYSES
PREPARATION OF HEXCALIBER TESTS AND PRELIMINARY THERMOMECHANICAL ANALYSES I. Ricapito a, G. Dell Orco b, P. A. Di Maio c, R. Giammusso c, A. Malavasi a, A. Tincani a, G. Vella c a ENEA C.R. Brasimone
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationExperimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 pebbles
Experimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 s D. Aquaro 1 N. Zaccari ABSTRACT Dipartimento di Ingegneria Meccanica Nucleare e della Produzione University of Pisa (Italy)
More informationDynamic Strain Aging, Negative StrainRate Sensitivity and Related Instabilities
TECHNISCHE MECHANIK, Band 3, Heft 4, (003), 160 166 Manuskripteingang: 14. Juli 003 Dynamic Strain Aging, Negative StrainRate Sensitivity and Related Instabilities A. Benallal, T. Borvik, A. Clausen,
More informationA multiscale approach for composite materials as multifield continua
Materials Science Forum Vols. 539543 (27) pp. 25512556 online at http://www.scientific.net (27) Trans Tech Publications, Switzerland A multiscale approach for composite materials as multifield continua
More informationDEFORMATION THEORY OF PLASTICITY
DEFORMATION THEORY OF PLASTICITY ROBERT M. JONES Professor Emeritus of Engineering Science and Mechanics Virginia Polytechnic Institute and State University Blacksburg, Virginia 240610219 Bull Ridge Publishing
More informationA Study on Modelling the Plane Strain Behaviour of Sand and its Stability
Archives of HydroEngineering and Environmental Mechanics Vol. 59 (2012), No. 3 4, pp. 85 100 DOI: 10.2478/heem20130001 IBW PAN, ISSN 1231 3726 A Study on Modelling the Plane Strain Behaviour of Sand
More informationForce and Stress. Processes in Structural Geology & Tectonics. Ben van der Pluijm. WW Norton+Authors, unless noted otherwise 1/9/ :35 PM
Force and Stress Processes in Structural Geology & Tectonics Ben van der Pluijm WW Norton+Authors, unless noted otherwise 1/9/2017 12:35 PM We Discuss Force and Stress Force and Units (Trigonometry) Newtonian
More informationAn alternative design method for the doublelayer combined die using autofrettage theory
https://doi.org/10.5194/ms82672017 Author(s) 2017. This work is distributed under the Creative Commons Attribution.0 License. An alternative design method for the doublelayer combined die using autofrettage
More information